Dimethyldichlorosilane Identifiers CAS number PubChem ChemSpider UNII Jmol-3D images Image 1 Properties Molecular formula C2H6Cl2Si Molar mass 129.06 g mol−1 Appearance clear liquid Density 1.064 g·cm−3 (l) Melting point
-76 °C, 197 K, -105 °F
70 °C, 343 K, 158 °F
Solubility in water Decomposes in water Hazards R-phrases S-phrases Flash point -9 °C (what is: /?)
Except where noted otherwise, data are given for materials in their standard state (at 25 °C, 100 kPa)
Dimethyldichlorosilane is a tetrahedral, organosilicon compound with the formula Si(CH3)2Cl2. At room temperature it is a colorless liquid that readily reacts with water to form both linear and cyclic Si-O chains. Dimethyldichlorosilane is made on an industrial scale as the principal precursor to dimethylsilicone and polysilane compounds.
The first organosilicon compounds were reported in 1863 by Charles Friedel and James Crafts who synthesized tetraethylsilane from diethylzinc and silicon tetrachloride. However, major progress in organosilicon chemistry did not occur until Kipping and his students began experimenting with diorganodichlorosilanes (R2SiCl2) that were prepared by reacting silicon tetrachloride with Grignard reagents. Unfortunately, this method suffered from many experimental problems.
In the 1930s, the demand for silicones increased due to the need for better insulators for electric motors and sealing materials for aircraft engines, and with it the need for a more efficient synthesis of dimethyldichlorosilane. To solve the problem, General Electric, Corning Glass Works, and Dow Chemical Company began a partnership that ultimately became the Dow Corning Company. During 1941-1942, Eugene G. Rochow, a chemist from General Electric, and Richard Müller, working independently in Germany, found an alternate synthesis of dimethyldichlorosilane that allowed it to be produced on an industrial scale. This Direct Synthesis, or Direct process, which is used in today’s industry, involves the reaction of elemental silicon with methyl chloride in the presence of a copper catalyst.
Rochow’s synthesis involved passing methyl chloride through a heated tube packed with ground silicon and copper(I) chloride. The current industrial method places finely ground silicon in a fluidized bed reactor at about 300 °C. The catalyst is applied as Cu2O. Methyl chloride is then passed through the reactor to produce mainly dimethyldichlorosilane.
- 2 CH3Cl + Si → (CH3)2SiCl2
The mechanism of the Direct Synthesis is not known. However, the copper catalyst is essential for the reaction to proceed.
In addition to dimethyldichlorosilane, products of this reaction include CH3SiCl3, CH3SiHCl2, and (CH3)3SiCl, which are separated from each other by fractional distillation. The yields and boiling points of these products are shown in the following chart.
Product Percent yield Bp (°C) (CH3)2SiCl2 80–90 70.0 CH3SiCl3 5–15 65.7 CH3SiHCl2 3–5 40.7 (CH3)3SiCl 3–5 57.3
Dimethyldichlorosilane hydrolyzes to form linear and cyclic silicones, compounds containing Si-O backbones. The length of the resulting polymer is dependent on the concentration of chain ending groups that are added to the reaction mixture. The rate of the reaction is determined by the transfer of reagents across the aqueous-organic phase boundary; therefore, the reaction is most efficient under turbulent conditions. The reaction medium can be varied further to maximize the yield of a specific product.
- n(CH3)2SiCl2 + nH2O → [(CH3)2SiO]n + 2nHCl
- m(CH3)2SiCl2 + (m+1)H2O → HO[Si(CH3)2O]mH + 2mHCl
Dimethyldichlorosilane reacts with methanol to produce dimethoxydimethylsilanes.
- (CH3)2SiCl2 + 2CH3OH → (CH3)2Si(OCH3)2 + 2HCl
- n(CH3)2Si(OCH3)2 + nH2O → [(CH3)2SiO]n + 2nCH3OH
Because dimethyldichlorosilane is easily hydrolyzed, it cannot be handled in air. One method used to overcome this problem is to convert it to a less reactive bis(dimethylamino)silane.
- (CH3)2SiCl2 + 4HN(CH3)2 → (CH3)2Si[N(CH3)2]2 + 2H2N(CH3)2Cl
- n(CH3)2Si[N(CH3)2]2 + nHO(CH2)2SiRSi(CH2)2OH → [(CH3)2SiO(CH2)2SiRSi(CH2)2O]n + 2nHN(CH3)2
Sodium metal can be used to polymerize dimethyldichlorosilane, producing polysilane chains with a Si-Si backbone. Other types of dichlorosilane monomers, such as Ph2SiCl2, can be added to adjust the properties of the polymer.
- n(CH3)2SiCl2 + 2nNa → [(CH3)2Si]n + 2nNaCl
- n(CH3)2SiCl2 + Ph2SiCl2 + 2(n+m)Na → [(CH3)2Si]n(Ph2Si)m + 2(n+m)NaCl
The main purpose of dimethyldichlorosilane is for use in the synthesis of silicones, an industry that, in 2005 was valued at more than 10 billion U.S. dollars per year. It is also employed in the production of polysilanes, which in turn are precursors to silicon carbide. In practical uses, dichlorodimethylsilane can be used as a coating on glass to avoid the adsorption of micro-particles.
- ^ a b Silicon: Organosilicon Chemistry. Encyclopedia of Inorganic Chemistry Online, 2nd ed.; Wiley: New Jersey, 2005. doi:10.1002/0470862106.ia220
- ^ a b Rochow, Eugene G (1950). "Dimethyldichlorosilane". Inorg. Synth. 3: 56–58. doi:10.1002/9780470132340.ch14.
- ^ a b c d Polysiloxanes and Polysilanes. Encyclopedia of Inorganic Chemistry Online, 2nd ed.; Wiley: New Jersey, 2005. DOI: 10.1002/0470862106.ia201
- ^ Ulrich Lauter,† Simon W. Kantor, Klaus Schmidt-Rohr, and William J. MacKnight, Vinyl-Substituted Silphenylene Siloxane Copolymers: Novel High-Temperature Elastomers. Macromolecules. 1999, 32, pp 3426-3431. DOI: 10.1021/ma981292f
- ^ Monjushiro, H. et al. "Size sorting of biological micro-particles by Newton-ring nano-gap device" Elsevier December 7, 2005
Wikimedia Foundation. 2010.
Look at other dictionaries:
dimethyldichlorosilane — noun A tetrahedral organosilicon compound used industrially as a precursor to dimethylsilicone and polysilane compounds … Wiktionary
Polysiloxane — Silicone Les silicones, ou polysiloxanes, sont des composés inorganiques formés d une chaine silicium oxygène (... Si O Si O Si O ...) sur laquelle des groupes se fixent, sur les atomes de silicium. Certains groupes organiques peuvent être… … Wikipédia en Français
Silicone — Les silicones, ou polysiloxanes, sont des composés inorganiques formés d une chaine silicium oxygène (... Si O Si O Si O ...) sur laquelle des groupes se fixent, sur les atomes de silicium. Certains groupes organiques peuvent être utilisés pour… … Wikipédia en Français
Silicones — Silicone Les silicones, ou polysiloxanes, sont des composés inorganiques formés d une chaine silicium oxygène (... Si O Si O Si O ...) sur laquelle des groupes se fixent, sur les atomes de silicium. Certains groupes organiques peuvent être… … Wikipédia en Français
Siloxane — The siloxane unit A siloxane is any chemical compound composed of units of the form R2SiO, where R is a hydrogen atom or a hydrocarbon group. They belong to the wider class of organosilicon compounds. Siloxanes can have branched or unbranched… … Wikipedia
Silicone — Not to be confused with the metalloid chemical element Silicon. Silicone caulk can be used as a basic sealant against water and air penetration. Silicones are inert, synthetic compounds with a variety of forms and uses. Typically heat resistant… … Wikipedia
DDS — Contents 1 Computer and information science 2 Electronics and Communications 3 Chemistry … Wikipedia
Peptide synthesis — In organic chemistry, peptide synthesis is the production of peptides, which are organic compounds in which multiple amino acids are linked via peptide bonds which are also known as amide bonds. The biological process of producing long peptides… … Wikipedia
Organosilicon — compounds are organic compounds containing carbon silicon bonds. Organosilicon chemistry is the corresponding science exploring their properties and reactivity. Like carbon, the organically bound silicon is tetravalent and tetrahedral. Carbon… … Wikipedia
List of Extremely Hazardous Substances — This is a list of Extremely Hazardous Substances as defined by Section 302 of the U.S. Emergency Planning and Community Right to Know Act. NOTOC A * Acetone cyanohydrin * Acetone thiosemicarbazide * Acrolein * Acrylamide * Acrylonitrile *… … Wikipedia